In vitro biological responses to nanofibrillated cellulose by human dermal, lung and immune cells: surface chemistry aspect
© The Author(s). 2017
Received: 7 July 2016
Accepted: 15 December 2016
Published: 10 January 2017
Nanocellulose, and particularly nanofibrillated cellulose (NFC), has been proposed for a diversity of applications in industry and in the biomedical field. Its unique physicochemical and structural features distinguish nanocellulose from traditional materials and enable its use as an advance nanomaterial. However, its nanoscale features may induce unknown biological responses. Limited studies with NFC are available and the biological impacts of its use have not been thoroughly explored. This study assesses the in vitro biological responses elicited by wood-derived NFC gels, when human dermal fibroblasts, lung MRC-5 cells and THP-1 macrophage cells are exposed to the nanomaterial. Furthermore, whether the presence of surface charged groups (i.e. carboxymethyl and hydroxypropyltrimethylammonium groups) on NFC can induce distinct biological responses is investigated.
The introduction of surface charged groups resulted in individual nanofibrils, while fibril aggregates predominated in the unmodified NFC gel suspensions as observed by transmission electron microscopy. In the presence of proteins, the surface modified NFCs formed compact agglomerates while the agglomeration pattern of the unmodified NFC was similar in the presence of proteins and in physiological buffer. Unmodified and modified NFC gels did not induce cytotoxicity in human dermal fibroblasts, lung and macrophage cells. No significant ROS production by THP-1 macrophages was found and no cellular uptake was observed. However, an inflammatory response was detected when THP-1 macrophages were treated with unmodified NFC as assessed by an increase in TNF-α and IL1-β levels, an effect that was absent when surface charged groups were introduced into NFC.
Taken together, the data presented here show the absence of cytotoxic effects associated with the exposure to unmodified, carboxymethylated and hydroxypropyltrimethylammonium-modified NFCs. Unmodified NFC presented a pro-inflammatory effect which can be further moderated by introducing surface modifications such as carboxymethyl and hydroxypropyltrimethylammonium groups into the nanofibrils. The present findings suggest that the inflammatory response to NFC might be driven by the material surface chemistry, and thus open up for the possibility of designing safe nanocellulose materials.
KeywordsCytotoxicity Inflammation Nanocellulose Surface chemistry
In recent years, an emerging demand for nano-based products from sustainable and environmental-friendly resources is placing nanocellulose on top of exciting nanomaterials near commercialization [1–4]. Nanocellulose consists of cellulose fibrils or crystallites with at least one dimension in the nanoscale and presents the typical physicochemical properties of cellulose such as hydrophilicity, mechanical strength and broad possibility of chemical modifications together with specific nanomaterial properties like high specific surface area and high aspect ratio [3, 4]. It can be derived from a diversity of sources, including wood, algae, bacteria and tunicates. Nanocellulose from wood and other higher plants is typically isolated as crystals (nanocellulose crystals) or nanofibrils (nanofibrillated cellulose (NFC)) through chemical and/or mechanical treatment of cellulose, while fibres of bacterial nanocellulose are produced by bacterial synthesis from low molecular weight sugars or other carbon sources [3–5].
Due to its novel physicochemical and structural features, nanocellulose has been proposed for a myriad of applications in industry (paper, packaging, electronics, cosmetics, etc.) and in the biomedical field, such as sensors and scaffolds for tissue engineering [6–10]. Although cellulose is considered as non-toxic, the novel physicochemical properties and nanoscale dimensions of nanocellulose may imply different biological effects from conventional cellulose [4, 5].
With the expected increase in the presence of nanocellulose in consumer products it is critical to assess and confirm the safety of the nanomaterial [8, 11]. Particularly, from an occupational point of view, potential hazard effects have been recently identified during the different life cycle stages of nanocellulose . During production and manufacturing of nanocellulose, two main potential hazards were identified, i) accidental inhalation of nanocellulose released to air after drying it and packaging it, and ii) dermal contact with slurry of nanocellulose when it is being combined with other materials, which can spill to the skin or clothes of the worker .
There is a void of knowledge concerning the effect of cellulose-based nanomaterials on human health . The in vitro studies available for nanocellulose, particularly for NFC, are mostly focus on exposure by inhalation with data from exposure via the dermal and oral routes still lacking . The few toxicological studies with NFC have so far shown no indication of toxicity [12–15]. However, different raw materials, manufacturing process and post-manufacturing chemical modifications may alter the material’s physicochemical properties . Properties like fibril dimensions, degree of crystallinity, specific surface area, degree of branching of the nanofibrils and modifications of the material chemical properties may affect the interactions between the cellulose nanofibrils and biological systems.
In the work presented here the focus is on NFC derived from wood and the potential occupational hazards derived from exposure to it. The aim is to evaluate the in vitro biological responses elicited by NFC, having in mind an occupational scenario and focusing on inhalation and dermal exposure routes. Whether chemical surface modifications of NFC could cause distinct biological responses is further investigated. Typically, surface charged groups are introduced during NFC production to facilitate the fibrillation process by adding repulsive charges . In this context, a side-by-side in vitro toxicity assessment of wood-derived NFC gels with different surface modifications (carboxymethylated and hydroxypropyltrimethylammonium-modified NFC) towards human dermal fibroblasts (HDF), lung MRC-5 cells and THP-1 macrophage cells is presented here, together with the evaluation of the cell responses to unmodified NFC.
Synthesis and surface modification of NFC
NFC was produced from commercial, never dried, bleached sulfite softwood dissolving pulp (Domsjö Fabriker AB, Sweden). Unmodified-NFC (U-NFC), carboxymethylated-NFC and hydroxypropyltrimethylammonium-NFC, here referred to as anionic NFC (A-NFC) and cationic NFC (C-NFC), in that order, were provided by Innventia AB (Sweden). U-NFC was prepared by enzymatic pretreatment of the pulp  while carboxymethylation and epoxypropyltrimethylammonium chloride (EPTMAC) quaternization pretreatments were used to prepare A-NFC and C-NFC respectively, as previously described . All samples were biocide free and showed no bacterial contamination when tested with 3 M™ Petrifilm™ bacteria tests (total aerobic count).
Transmission electron microscopy
The morphology of the fibres in phosphate buffer and in cell culture medium was investigated by transmission electron microscopy (TEM). Samples were prepared as described by Usov et al. . Briefly, 5 μl of NFC stock solution (in PBS) were deposited onto carbon-coated copper grids (400 mesh), while 5 μl of NFC in RPMI cell culture medium (500 μg/ml, prepared as described below) were placed on formvar coated 200 mesh copper grids. After adsorption, the sample grids were stained with 2% uranyl acetate to achieve a noncrystalline film of stain embedding the fibres. Following the staining step, the excess moisture was drained along the periphery using filter paper. Dried grids were examined using TEM (FEI Tecnai G2) operated at 100 kV or at 80 kV.
ζ – potential
Dispersions of 0.001% (w/w) of the NFC samples were prepared in 10 mM NaCl and in cell culture media, DMEM and RPMI1640 (ThermoFisher Scientific), through ultrasonication for 30 s (Vibracell 600 W, 20 kHz). The electrophoretic mobility of the samples was measured using a universal dip cell in a ZetaSizer Nano instrument (Malvern Instruments) at 25 °C and 37 °C (in the case of cell culture media). The ζ-potentials were determined from the electrophoretic mobility applying the Smoluchowski equation .
Preparation of NFC exposure suspensions
Stock solutions of U-NFC, A-NFC and C-NFC were prepared in phosphate buffer (PBS) at 5 mg/mL and dispersed with an ultrasonic probe (Vibracell 600 W, 20 kHz) during 12 min. The final stock solutions were sterilized by autoclaving, except for C-NFC which was subject to ultraviolet radiation (UV) treatment during two cycles of 45 min each. Before each exposure, the stock solutions were diluted in cell culture media (concentration range 50 to 500 μg/mL) and sonicated for 30 min in a water bath sonicator (Bransonic 3510) before being added to the cells.
The human dermal fibroblasts (HDF) from European Collection of Authenticated Cell Cultures (ECACC), the human MRC-5 lung fibroblast cell line (private collection), and the human THP-1 monocytic cell line (ECACC) were used in this study. MRC-5 and HDF cells were cultured in DMEM/F12 medium (ThermoFisher Scientific), and THP-1 cells in RPMI 1640 medium (ThermoFisher Scientific) supplemented with 10% (v/v) heat-inactivated fetal bovine serum (FBS), 100 IU/mL penicillin and 100 μg/mL streptomycin (both from ThermoFisher Scientific). The cells were incubated in a humidified atmosphere at 37 °C, 5% CO2 and sub-cultured at 70–80% confluency.
For each experiment, HDF and MRC-5 cells were seeded in 96 well-plates at a density of 6 × 103 cells/well (200 μl/well) 1 day prior to NFC treatment. THP-1 monocytes were seeded in 96 well-plates at a density of 2.5 × 104 cells/well (200 μl/well) and differentiated into macrophages using 5 ng/mL phorbol myristate acetate (PMA) (Sigma-Aldrich) for 48 h before NFC treatment .
Near confluent monolayers of HDF and MRC-5 cells, and THP-1 differentiated macrophages were finally exposed to U-NFC, A-NFC and C-NFC at concentrations ranging from 50 to 500 μg/mL in 96-well plate (200 μl/well) for 24 h. Food grade microcrystalline cellulose (MCC, Avicel® CL-611, 100 nm in diameter microcrystals mixed with soluble sodium carboxymethylcellulose, FMC Biopolymer) was used as reference material. As a positive control, 5% (w/w) dimethyl sulfoxide (DMSO) (Sigma-Aldrich) in cell culture medium was used, while non-treated cells served as negative control.
Cellular metabolic activity: Alamar Blue assay
The alamar blue (AB) assay was used to assess cellular metabolic activity as a marker of cytotoxicity. After exposure to NFC, cells were carefully washed with 100 μL warm PBS, and 200 μL of Alamar Blue® reagent (ThermoFisher Scientific) diluted (1:10) was added to each well and incubated for 90 min at 37 °C. After incubation, 100 μL of each well were collected and added to a black 96-well plate. The fluorescence was measured at 560 nm excitation and 590 nm emission wavelengths using a plate reader (Tecan Infinite M200). Results were expressed as percentage of cell viability with respect to the negative control. The experiments were performed at least three times in triplicate wells for each dose. Interference of the NFC samples with the assay was tested in an acellular system by incubating different doses of NFC with the AB reagent for 90 min at 37 °C in 96 well plates. Cell culture media interference was also measured. Neither NFC samples nor the cell culture media interfere with the AB assay.
Cellular membrane integrity: Lactate Dehydrogenase assay
The release of the intracellular enzyme lactate dehydrogenase (LDH), indicative of cell membrane damage, was assessed by a LDH kit (Abcam) according to the manufacturer’s guidelines. Briefly, after cell exposure to the NFC samples, cell culture supernatants were collected and adherent cells were lysated for 30 min with cell lysis buffer diluted in cell culture medium (1:10) and the lysates were collected. Lysates and supernatants were centrifuged at 6800 g during 10 min to avoid any potential interference of NFC. The enzyme activity in the lysates and supernatants samples was measured by reading the absorbance at 450 nm wavelength and reference wavelength 650 nm using a plate reader (Tecan Infinite M200). The experiments were conducted at least three times in duplicate wells for each dose. LDH release (LDH activity in cell culture supernatant) was normalized by the total LDH activity (sum of LDH activity in cell culture supernatants and lysates) which correlates with the total number of cells in order to avoid any underestimation of toxicity .
Cell morphology - Light microscopy
After 24 h exposure to NFC, cells were carefully rinsed with warm PBS and observed under light microscopy (Nikon Eclipse TE2000-U) to evaluate their morphology.
The inflammatory response was investigated by quantifying the secreted levels of the cytokines tumor necrosis factor α (TNF-α) and interleukin 1 beta (IL1-β). THP-1 monocytes were differentiated into macrophages and treated with the NFC suspensions as described above. After 24 h exposure, cell culture supernatants were collected, centrifuged at 6800 g during 10 min and further analyzed for the levels of cytokines using ELISA Kits (human TNF-α and human IL1-β ELISA Kits, Thermo Fischer Scientific) according to the manufacturer’s protocol. As a positive control for TNF-α and IL1-β induction, cells were treated with lipopolysaccharide (LPS) from Pseudomonas aeruginosa at 1 ng/mL. The same experiments were performed in the presence of polymyxin B (PMB) at a final concentration of 25 μg/mL in order to inhibit the potential effects of any endotoxin present in the NFC samples . The experiments were conducted at least three times in duplicate wells for each dose. TNF-α and IL1-β concentrations were calculated from a standard curve plotted for each experiment.
Reactive oxygen species production
The levels of intracellular reactive oxygen species (ROS) were measured using the dichlorodihydrofluorescein diacetate (DCFH-DA) assay (Abcam) according to the manufacturer’s guidelines. DCFH-DA is a lipophilic cell permeable compound that is deacetylated in the cytoplasm by cellular esterases, and later oxidized by ROS to a highly fluorescent molecule. THP-1 monocytes were differentiated into macrophages and loaded with 20 μM DCFH-DA in PBS for 30 min at 37 °C. Thereafter, cells were treated with the NFC suspensions (50, 100, 250 500 μg/mL) and fluorescence was recorded every 30 min over 120 min (excitation 485 nm, emission 535 nm) at 37 °C using a plate reader (Tecan Infinite M200). Tert-butyl hydroperoxide (TBHP, 50 μM) was used as positive control.
Cellular uptake of NFC - Transmission electron microscopy
TEM was used to investigate if the NFC materials were uptaken by THP-1 macrophages. THP-1 macrophages were exposed to the different NFC samples (500 μg/ml) for 24 h and then fixed in 2.5% (v/v) glutaraldehyde overnight at 4 °C. Samples were washed with sodium cacodylate buffer and subsequently post-fixed with 1% osmium tetroxide in sodium cacodylate buffer. Afterwards, the cells were dehydrated in ascending ethanol series, embedded in epon and finally polymerized at 60 °C for 48 h. From the embedded cells, ultrathin sections (50–60 nm) were cut parallel to the vertical axis of the inserts, mounted on copper grids and stained with uranyl acetate and lead citrate. Imaging was done with a Technai G2 microscope (FEI, Netherlands) LaB6 filament at 80 kV.
Data analysis was conducted using GraphPad Prism 6, version 6.07 (GraphPad Software Inc., La Jolla, USA) by one-way or two-way analysis of variance (ANOVA) followed by Dunnett’s multiple comparison post-hoc tests. p-values lower than 0.05 were considered statistically significant. Results are presented as the mean ± standard error of the mean (SEM).
Physico-chemical characteristics of the NFC samples under study
Content of functional groups (mmol/g) a
Degree of crystallinityb (%)
Fibre diameter (in PBS) c
20–30 nm fibril aggregates
−11.3 ± 1.3
−4.0 ± 0.2
−5.2 ± 0.6
4–5 nm individual fibrils
−34.1 ± 1.7
−12.7 ± 2.7
−12.6 ± 1.6
4–5 nm individual fibrils
24.2 ± 2.0
−7.2 ± 2.9
−8.1 ± 2.0
The successful introduction of carboxymethyl and hydroxypropyltrimethylammonium groups on A-NFC and C-NFC, respectively, was previously verified by Hua et al. . Results showed a higher surface group density for C-NFC than for A-NFC. No specific surface groups were introduced during the production of U-NFC (mild enzymatic pretreatment of the wood pulp) and thus only low levels of carboxyl group content could be expected due to the presence of residual hemicellulose. Furthermore, the degree of crystallinity, as previously determined , was similar between both unmodified and modified NFCs indicating that the chemical modifications did not considerably alter the crystallinity of NFC.
Zeta potential was measured for all NFCs. At pH 7.4, A-NFC and C-NFC suspended in 10 mM NaCl presented zeta potential values of − 34.1 and 24.2 mV, respectively, confirming the presence of the negatively and positively charged groups in the modified NFCs. The high absolute values of zeta potential for the charged samples implies a good stability of the suspensions . However, U-NFC formed an unstable dispersion, showing tendency to aggregate, with a slightly negative surface charge (−11.3 mV). When incubated in cell culture media and at 37 °C, all NFCs samples showed negative zeta potential values in the range of − 4 and − 12 mV, independently of the cell culture medium used.
NFCs are not cytotoxic for immune, dermal and lung cells
The AB assay showed that after 24 h exposure, the metabolic activity of the treated cells was comparable to the activity of the non-treated cells (negative control) for the HDF and MRC-5 cells (Fig. 3a and b). Interestingly, THP-1 cells showed a significantly higher metabolic activity of the NFC-treated cells compared with the negative control (Fig. 3c), an effect that has been also observed by other authors when exposing macrophages to NFC .
No signs of toxicity were observed when the LDH assay was used to evaluate cell membrane damage following 24 h treatment with NFCs (Fig. 4). HDF cells exposed to NFCs with or without surface modifications did not significantly change the LDH release when compared to the negative control (Fig. 4a). Moreover, no significant differences in total cell number (total LDH) between treated and non-treated cells were found. The MRC-5 cells and THP-1 macrophages showed a similar pattern of LDH release and total LDH to the results found for HDF cells (Fig. 4b and c, respectively). The reference material MCC was also not cytotoxic for the studied cells under the conditions of the present work.
U-NFC induces the release of pro-inflammatory cytokines
U-NFC triggered a significant release of IL1-β by THP-1 macrophages at the two high doses, 250 and 500 μg/mL (Fig. 6b ). Both modified NFCs, A- and C-NFC, did not induce IL1-β secretion. MCC did not induce production of any of the pro-inflammatory cytokines under study.
No intracellular ROS increase upon treatment with NFCs
THP-1 macrophages do not uptake the NFC materials
The TEM analysis of the cells after exposure to the different NFC materials confirmed that there were no alterations in cell morphology and showed that none of the NFC samples were uptaken by the THP-1 macrophages. No signs of phagocytosis attempts were found. Representative TEM images of THP-1 macrophages after 24 h exposure to the different NFC materials at a concentration of 500 μg/ml, together with images of the non-treated cells can be found in the supplementary information (Additional file 4: Figure S4).
In this study, the toxicity impacts of unmodified and surface modified NFC gels (i.e. carboxymethylated and hydroxypropyltrimethylammonium-substituted NFC) on dermal, lung and macrophage cells were compared for the first time. The selected human cell types represent cells most likely to be impacted by the potential exposure to NFC in an occupational setting, including immune surveillance and epithelial cells covering the respiratory tract and the skin.
Surface charges are introduced during the preparation of nanocellulose where adding repulsive charges facilitates the defibrillation process. As expected, the presence of surface charged groups in A-NFC and C-NFC and the subsequent electrostatic repulsion between fibres resulted in individual nanocellulose fibrils, while fibres tended to aggregate in the low carboxyl group content U-NFC. The zeta potential further confirmed the different surface charges of the studied samples, however in the presence of cell culture medium all samples showed slightly negative charge (zeta potential values between − 4 and − 12 mV). As described for other nanomaterials, the nanofibres may be rapidly covered by the biomolecules present in the cell culture medium, forming a biomolecular corona that partially or fully covers the nanofibers and mask the surface charge and, consequently, changes the zeta potential [26, 27].
The effect of protein adsorption was also reflected in the agglomeration pattern of A-NFC and C-NFC, which drastically changed from dispersed fibres in phosphate buffer to compact agglomerates in cell culture medium. As also observed by Tomic et al. , the agglomeration of U-NFC did not significantly change when comparing cell culture medium and phosphate buffer suspensions, showing the presence of small agglomerates in both conditions. The type, amount and conformation of the adsorbed proteins will be influenced by the nanofibre surface chemistry among other nanomaterials properties. In turn, the different protein adsorption patterns may promote distinct agglomeration states of the nanomaterial , as reflected here.
The assessment of potential toxic effects showed that the NFC materials under study did not have any impact on the metabolic activity or on the membrane integrity of the treated cells following 24 h exposure. Overall, the NFCs under study did not impair the cell viability of dermal, lung or macrophage cells. This is in accordance with previous in vitro studies showing that NFC gels are non- cytotoxic for a wide range of cells, including dendritic cells, macrophages, fibroblasts, keratinocytes, human cervic carcinoma and hepatoma cell lines [13–15, 28]. Moreover, NFC gels, aerogels and membranes were proven to be biocompatible when evaluated for diverse tissue engineering and biomedical applications [12, 18, 30–33].
Furthermore, no significant ROS production by THP-1 macrophages was found under the conditions tested in the present work. However, it was shown that U-NFC promoted an inflammatory response in terms of secretion of TNF-α and IL-1β, a response that was suppressed when surface charges were introduced on the nanofibrils.
It is well-known that the inhalation of toxic airborne particulates, particularly carbon nanotubes and other fibre-like nanomaterials can cause pulmonary inflammation . Macrophages play a critical role in the recognition, and clearance of pathogens and foreigner particulates. The acute phase responses to inhaled particulates are described by a pulmonary inflammation set by the release of a number of inflammatory mediators, such as TNF-α and IL1-β. These two cytokines, TNF-α and IL1-β, acting synergistically, are involved in the pathogenesis of various acute and chronic respiratory diseases .
The secretion of pro-inflammatory cytokines by macrophages under the influence of NFC has been previously investigated in vitro and in vivo. While some authors showed that NFC gels were non pro-inflammatory in vitro [13, 15, 24, 31], Catalán and co-workers found a pro-inflammatory response to NFC in vivo . However, the authors declared that the possible role of microbial contamination on the inflammatory effect could not be ruled out. Interestingly, when we have previously studied the pro-inflammatory response of THP-1 monocytes cultured on NFC films we found a pro-inflammatory effect with U-NFC and A-NFC, while C-NFC behaved as an inert material . Thus, a pro-inflammatory effect was found when carboxymethyl groups (A-NFC) were introduced on the nanofibrils, an effect that was absent in the present work. Such difference in the inflammatory response of A-NFC could be partially due to the variations in the structures of the nanocelluloses under study, i.e. gels versus membranes, and in how the cells were exposed to the materials.
Hypothetical cellular mechanisms of inflammation caused by fibres include i) frustrated phagocytosis and the subsequent production of ROS and oxidative stress or ii) a direct effect of the fibres on the membrane receptors . ROS production was not found when macrophages were incubated with the NFC gels studied here and TEM analysis of the exposed cells revealed no sings of phagocytosis attempts, with untreated cells and NFC-exposed cells showing comparable morphologies. Besides, it was not possible to detect the presence of any of the NFC materials inside the cells. Therefore, we hypothesize that the observed secretion of pro-inflammatory cytokines is likely a consequence of fibre-receptor interactions, where surface chemistry plays a key role. Surface chemistry influences the type, conformation and amount of adsorbed proteins which in turn mediate the cell-nanomaterial interactions . It can be speculated that the protein corona of U-NFC might promote the interaction with THP-1 membrane receptors resulting in the secretion of pro-inflammatory cytokines. However, the presence of carboxymethyl and hydroxypropyltrimethylammonium groups on A-NFC and C-NFC, respectively, most probably result in protein coronas that do not promote the signalling for an inflammatory effect. Besides, surface chemistry and the subsequent protein adsorption might also indirectly affect the cellular response to the nanomaterial by impacting on its agglomeration pattern . The difference in surface chemistry, particularly in surface charges, was indeed reflected in the agglomeration patterns of the NFC materials and therefore an effect of nanofibre dispersion on the observed inflammatory response cannot be dismissed. Authors have described the influence of fibre agglomerates in in vivo cellular responses of nanofibres such as carbon nanotubes and carbon fibres [38, 39]. Mutlu et al. showed that the aggregation of single-walled carbon nanotubes accounted for its pulmonary toxicity, an effect that could not be seen when the carbon nanotubes were nanoscale dispersed . Nevertheless, in the present study, U-NFC with smaller agglomerates compared with A-NFC and C-NFC was the material that promoted a pro-inflammatory response and macrophages did not react differently to the diverse agglomerate sizes in terms of frustrated phagocytosis or cellular uptake.
The cellular uptake of NFC has recently been investigated by other authors [28, 36]. Catalán et al. administrated TEMPO-oxidized NFC (negatively charged NFC) to mice by pharyngeal aspiration and reported dose-related accumulation of the material in the cytoplasm of macrophages . Conversely to our work, in vitro studies with dendritic cells showed partial internalization of NFC . The authors stated that the interaction of NFC and the dendritic cells depended on the thickness and length of the material and highlight the need of further studies to investigate the mechanism that predominate in the NFC-dendritic cells interactions .
In summary, the findings presented here suggest that the inflammatory response to NFC gels might be driven by the surface chemistry. Furthermore, the fact that U-NFC induces an inflammatory response under no signs of toxicity may pose a concern and indicates that, as also observed by others, cytotoxicity and activity (e.g. inflammatory response) do not necessary correlate . Understanding the effect of NFC features, in this case, the surface chemistry on their biological reactivity will contribute towards safer industrial applications of such nanomaterial. More studies are needed, especially for prolonged exposure times and in vivo tests, to further investigate the effect of NFC on the immune response and enhance our present knowledge about the safety of nanocelluloses.
No indication of cytotoxicity or significant ROS production were found when cells were exposed to the unmodified and surface modified NFC gels. Besides, no cellular uptake was observed. A pro-inflammatory response with U-NFC in terms of cytokine secretion was found and this effect was suppressed when surface charged groups were present on the nanofibrils. This finding suggests that the inflammatory response to NFC gels might be driven by surface chemistry opening up the possibility for the design of safe nanocellulose materials.
Anionic nanofibrillated cellulose
Analysis of variance
Cationic nanofibrillated cellulose
Dulbecco’s Modified Eagle Medium: Nutrient Mixture F-12
European Collection of Authenticated Cell Cultures
Interleukin 1 beta
Phorbol myristate acetate
Reactive oxygen species
- RPMI 1640:
Roswell Park Memorial Institute (RPMI) 1640 Medium
Standard error of the mean
Transmission electron microscopy
Tumor necrosis factor α
Unmodified cellulose nanofibrillated
The authors would like to thank Ida-Maria Sintorn and Lars Haag (Vironova), Vironova AB (Stockholm) and SciLifeLab BioVis Facility, Uppsala University for the TEM images acquisition. Monica Johnson is acknowledged for assistance in the experimental work with MRC-5 cells. Eva Ålander and Tom Lindström at Innventia AB are acknowledged for supplying the nanocellulose materials and for valuable discussions. Alex Basu at the Division of Nanotechnology and Functional Materials, Uppsala University is acknowledged for imaging processing.
This study was financially supported by FORMAS (Project No. 2014–151), Lars Hierta Minne Foundation (Project No. FO2014-0437), Olle Byggmästare Foundation (Project No. 2014/457) and European Union’s Seventh Framework Programme (FP7/2007-2013) under grant agreement No. 604387 (GUIDEnano).
Availability of data and material
The data supporting our conclusions is included in the main body of the manuscript or in the Additional files.
VRL participated in the design of the study, carried out all the cellular experiments (except AB assay for HDF cells), performed the statistical analysis, data interpretation and wrote the manuscript. CS performed part of the in vitro experiments with HDF cells and the initial experiments with THP-1 cells. MS participated in the planning of the study and the evaluation of the results. NF participated in the design of the study, carried out the cellular uptake studies, did the data interpretation and wrote the manuscript together with VRL. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Consent for publication
Ethics approval and consent to participate
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
- Azizi Samir MAS, Alloin F, Dufresne A. Review of recent research into cellulosic whiskers, their properties and their application in nanocomposite field. Biomacromolecules. 2005;6(2):612–26.View ArticlePubMedGoogle Scholar
- Eichhorn SJ, Dufresne A, Aranguren M, Marcovich NE, Capadona JR, Rowan SJ, et al. Review: Current international research into cellulose nanofibres and nanocomposites. J Mater Sci. 2010;45:1.View ArticleGoogle Scholar
- Moon RJ, Martini A, Nairn J, Simonsen J, Youngblood J. Cellulose nanomaterials review: Structure, properties and nanocomposites. Chem Soc Rev. 2011;40:7.View ArticleGoogle Scholar
- Dufresne A. Nanocellulose: a new ageless bionanomaterial. Mater Today. 2013;16(6):220–7.View ArticleGoogle Scholar
- Klemm D, Kramer F, Moritz S, Lindström T, Ankerfors M, Gray D, et al. Nanocelluloses: A New Family of Nature-Based Materials. Angew Chem Int Ed Engl. 2011;50:24.View ArticleGoogle Scholar
- Johansson C, Bras J, Mondragon I, Nechita P. Renewable fibers and bio-based materials for packaging applications–a review of recent developments. Bioresources. 2012;7:2.View ArticleGoogle Scholar
- Jorfi M, Foster EJ. Recent advances in nanocellulose for biomedical applications. J Appl Polym Sci. 2015;132:14.View ArticleGoogle Scholar
- Shatkin JA, Kim B. Cellulose nanomaterials: life cycle risk assessment, and environmental health and safety roadmap. Environ Sci: Nano. 2015;2:5.Google Scholar
- Siró I, Plackett D. Microfibrillated cellulose and new nanocomposite materials: a review. Cellulose. 2010;17:3.View ArticleGoogle Scholar
- Lin N, Dufresne A. Nanocellulose in biomedicine: Current status and future prospect. Eur Polym J. 2014;59.
- Lindström T, Aulin C, Naderi A, Ankerfors M. Microfibrillated Cellulose. John Wiley & Sons. 2014. p. 1.Google Scholar
- Alexandrescu L, Syverud K, Gatti A, Chinga-Carrasco G. Cytotoxicity tests of cellulose nanofibril-based structures. Cellulose. 2013;20:4.View ArticleGoogle Scholar
- Čolić M, Mihajlović D, Mathew A, Naseri N, Kokol V. Cytocompatibility and immunomodulatory properties of wood based nanofibrillated cellulose. Cellulose. 2014;22:1.Google Scholar
- Pitkänen M, Kangas H, Laitinen O, Sneck A, Lahtinen P, Peresin MS, et al. Characteristics and safety of nano-sized cellulose fibrils. Cellulose. 2014;21:6.View ArticleGoogle Scholar
- Vartiainen J, Pöhler T, Sirola K, Pylkkänen L, Alenius H, Hokkinen J, et al. Health and environmental safety aspects of friction grinding and spray drying of microfibrillated cellulose. Cellulose. 2011;18:3.View ArticleGoogle Scholar
- Lavoine N, Desloges I, Dufresne A, Bras J. Microfibrillated cellulose – Its barrier properties and applications in cellulosic materials: A review. Carbohydr Polym. 2012;90:2.View ArticleGoogle Scholar
- Pääkkö M, Ankerfors M, Kosonen H, Nykänen A, Ahola S, Österberg M, et al. Enzymatic Hydrolysis Combined with Mechanical Shearing and High-Pressure Homogenization for Nanoscale Cellulose Fibrils and Strong Gels. Biomacromolecules. 2007;8:6.View ArticleGoogle Scholar
- Hua K, Carlsson DO, Alander E, Lindstrom T, Stromme M, Mihranyan A, et al. Translational study between structure and biological response of nanocellulose from wood and green algae. RSC Adv. 2014;4:6.Google Scholar
- Usov I, Nystrom G, Adamcik J, Handschin S, Schutz C, Fall A, et al. Understanding nanocellulose chirality and structure-properties relationship at the single fibril level. Nat Commun. 2015;6:7564.View ArticlePubMedPubMed CentralGoogle Scholar
- White B, Banerjee S, O’Brien S, Turro NJ, Herman IP. Zeta-potential measurements of surfactant-wrapped individual single-walled carbon nanotubes. J Phys Chem C. 2007;111:37.View ArticleGoogle Scholar
- Park EK, Jung HS, Yang HI, Yoo MC, Kim C, Kim KS. Optimized THP-1 differentiation is required for the detection of responses to weak stimuli. Inflamm Res. 2007;56:1.View ArticleGoogle Scholar
- Stone V, Johnston H, Schins RPF. Development of in vitro systems for nanotoxicology: methodological considerations. Crit Rev Toxicol. 2009;39:7.View ArticleGoogle Scholar
- Duff GW, Atkins E. The inhibitory effect of polymyxin B on endotoxin-induced endogenous pyrogen production. J Immunol Methods. 1982;52:3.Google Scholar
- Hua K, Ålander E, Lindström T, Mihranyan A, Strømme M, Ferraz N. Surface Chemistry of Nanocellulose Fibers Directs Monocyte/Macrophage Response. Biomacromolecules. 2015;16:9.View ArticleGoogle Scholar
- Riddick T. Control of colloid stability through zeta potential: with a closing chapter on its relationship to cardiovascular disease. vol. 1. New York: Livingston Publishing Company; 1968.Google Scholar
- Lesniak A, Salvati A, Santos-Martinez MJ. Nanoparticle adhesion to the cell membrane and its effect on nanoparticle uptake efficiency. J Am Chem Soc. 2013;135:4.View ArticleGoogle Scholar
- Forest V, Cottier M, Pourchez J. Electrostatic interactions favor the binding of positive nanoparticles on cells: A reductive theory. Nano Today. 2015;10(6):677–80.View ArticleGoogle Scholar
- Tomic S, Kokol V, Mihajlovic D, Mircic A, Colic M. Native cellulose nanofibrills induce immune tolerance in vitro by acting on dendritic cells. Sci Rep. 2016;6:31618.View ArticlePubMedPubMed CentralGoogle Scholar
- Fubini B, Ghiazza M, Fenoglio I. Physico-chemical features of engineered nanoparticles relevant to their toxicity. Nanotoxicology. 2010;4:347–63.View ArticlePubMedGoogle Scholar
- Bhattacharya M, Malinen MM, Lauren P, Lou Y-R, Kuisma SW, Kanninen L, et al. Nanofibrillar cellulose hydrogel promotes three-dimensional liver cell culture. J Control Release. 2012;164:3.View ArticleGoogle Scholar
- Kollar P, Závalová V, Hošek J, Havelka P, Sopuch T, Karpíšek M, et al. Cytotoxicity and effects on inflammatory response of modified types of cellulose in macrophage-like THP-1 cells. Int J Immunopharmacol. 2011;11:8.Google Scholar
- Lou Y-R, Kanninen L, Kuisma T, Niklander J, Noon LA, Burks D, et al. The Use of Nanofibrillar Cellulose Hydrogel As a Flexible Three-Dimensional Model to Culture Human Pluripotent Stem Cells. Stem Cells Dev. 2014;23:4.View ArticleGoogle Scholar
- Zander NE, Dong H, Steele J, Grant JT. Metal cation cross-linked nanocellulose hydrogels as tissue engineering substrates. ACS Appl Mater Inter. 2014;6:21.View ArticleGoogle Scholar
- Donaldson K, Poland CA, Murphy FA, MacFarlane M, Chernova T, Schinwald A. Pulmonary toxicity of carbon nanotubes and asbestos — Similarities and differences. Adv Drug Deliv Rev. 2013;65:15.View ArticleGoogle Scholar
- Dinarello CA. Proinflammatory cytokines. Chest. 2000;118:2.View ArticleGoogle Scholar
- Catalan J, Rydman E, Aimonen K, Hannukainen KS, Suhonen S, Vanhala E, et al. Genotoxic and inflammatory effects of nanofibrillated cellulose in murine lungs. Mutagenesis. 2016. doi:10.1093/mutage/gew035.PubMedGoogle Scholar
- Donaldson K, Tran LC. Inflammation caused by particles and fibers. Inhal Toxicol. 2002;14:1.View ArticleGoogle Scholar
- Murray AR, Kisin ER, Tkach AV, Yanamala N, Mercer R, Young SH, et al. Factoring-in agglomeration of carbon nanotubes and nanofibers for better prediction of their toxicity versus asbestos. Part Fibre Toxicol. 2012;9:10.View ArticlePubMedPubMed CentralGoogle Scholar
- Mutlu GM, Budinger GR, Green AA, Urich D, Soberanes S, Chiarella SE, et al. Biocompatible nanoscale dispersion of single-walled carbon nanotubes minimizes in vivo pulmonary toxicity. Nano Lett. 2010;10:5.View ArticleGoogle Scholar
- Xia T, Hamilton RF, Bonner JC, Crandall ED, Elder A, Fazlollahi F, et al. Interlaboratory evaluation of in vitro cytotoxicity and inflammatory responses to engineered nanomaterials: the NIEHS Nano GO Consortium. Environ Health Perspect. 2013;121:6.View ArticleGoogle Scholar